Fabrication and electrical characteristic of quaternary ultrathin hf tiero thin films for mos devices grown by rf sputtering
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201341Fabrication and Electrical characteristic of quaternaryultrathin HfTiErO thin films for MOS devices grown by rfsputteringMurad Ali Khaskheli1,4,Ping Wu1*, Amir Mahmood Soomro3, Matiullah Khan2Mujtaba Ellahi2,Asadullah2,Mohammad Siddique Kalhoro41. School of Mathematics and Physics, University of Science and Technology Beijing 100083, PR China2. School of Material sciences and Engineering , University of Science and Technology Beijing 100083, PRChina3. School of Automation, Beijing Institute of Technology, Beijing 100081, P. R. China4. Institute of Physics, University of Sindh, Jamshoro, Pakistan* E-mail of the corresponding author: email@example.comAbstractUltra-thin Ti and Er co-doped HfO2 films were grown on Si substrate by RF sputtering at different compositions andsubjected to rapid thermal annealing at 500 °C and 700 °C in nitrogen ambient for 60 s. Dielectric properties ofultrathin co doped with Tritium and Erbium into hafnium oxide (HfO2) with rapid thermal annealing (RTA) havebeen investigated. Ti and Er different contents doped HfO2 thin films about (5 to 10) nm thicknesses have beenemployed for Au/HfTiErO/Si/Au metal oxide semiconductor (MOS) structures fabrication. The fabricated MOS(Au/HfTiErO/Si/Au) structure has been used for extracting electrical properties such that, dielectric constant,effective charge carriers, flat band voltage, interface trap density and doping concentration through capacitancevoltage measurements. The films compared at different contents used for Ti and Er doped with HfO2 on growthparameters, which could not showed excellent properties due to small thickness and other several defects during thedepositions. While, the film annealed at 500 °C has the improved microstructure and electrical characteristics.Furthermore Atomic force microscopy and X-ray photo electron microscopy analysis verified the microstructure ofHfTiErO gate oxide for future MOS devices.Keywords: high-k, HfTiErO, Thin films, rf Sputtering1. IntroductionIn order to resolve the problem of device compatibility, reliability and high gate leakage currents, Recently, high-k gate dielectrics are explored to replace conventional SiO2 as an alternative gate dielectric materials(Schaller et al.,2004). There are several high-k dielectric material have been introduced to replace it one the suitable material isHfO2, which has been considered a suitable high-k gate dielectrics material for integration in complementary metaloxide semiconductor (CMOS) devices because of its good thermal stability and wide band gap on Si (Wilk et al.,2001). Unfortunately, besides the merits, there are several drawbacks of HfO2 ZrO2, Al2O3 and Y2O3 (Akbar et al.,2003) (Mikhelashvili et al., 2001) (Buchanan et al., 1999) dielectric materials. All these materials have a very lowcrystallization onset temperature on silicon, which caused the formation of interfacial layers often occurs. However,it was also observed that the mobility reduces when the Vfb of hafnium oxide shifts with the increasing of EOT. Thedegradation of Vfb and poor mobility are the results of crystallization, which produces the oxygen vacancies in theinterfacial layer and in the high k layers when these materials are deposited on Si. The existence of any interfaciallayer of silicate material or silicon dioxide will limit the highest possible gate stack capacitance and produce avariation of electrical properties(Yamamoto et al., 2006). Moreover, the occurrence interfacial layer on dielectric/Siwhich degrade the device performance. To attain new aggressive scaling, recently hafnium based dielectricsmaterials have been proposed for the next generations (Chen et al., 2004) (Auciello, et al 2005). it has been reportedthat doping of Er, Dy, Nd, or Tb or TiOx into hafnium oxide dielectric films showed excellent electricalcharacteristics (Först et al., 2005) ( Klie et al., 2003) and the physical properties were investigated by using x-rayphotoelectron spectroscopy (XPS) (Kim et al., 2004). However, the electrical, dielectric, microstructure and optical,properties of ultrathin films depend strongly on the growth conditions fabrication process, and post depositionannealing treatment.A number of methods and deposition techniques have been employed to attain fine quality of high-k thin films, forinstance chemical vapor deposition (CVD), molecular beam-epitaxy (MBE) atomic layer deposition (ALD) , reactivethermal evaporation and pulsed-laser deposition (PLD) etc (Dey et al., 2004) (Park et al., 2002) (He et al., 2007)
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201342(Ergin et al., 2010). Although RF sputtering (Ergin et al., 2010) is PVD based technique combined with plasmaoffers a low temperature processing and blocks the oxygen from the ambience, which prevents the formation ofinterfacial layer (IL). Therefore, in this work RF sputtering technique explores the possibility of obtaining the goodquality high-k gate dielectric thin films, which is the most important requirement of advanced CMOS technology.In the present study, HfO2-based thin layers have been fabricated by RF magnetron sputtering of a pure HfO2 with Tiand different Er targets in pure argon plasma. The fabrication and electrical properties of the ultrathin films havebeen analyzed by means of such as atomic force microscopy (AFM), X-ray photoelectron spectroscopy (XPS) andcapacitance-voltage (C-V) with respect to the deposition conditions and the annealing treatments. A special focus ofthe study is to reveal the relationship between Er-doped content and the surface roughness, chemical compositionsand electrical properties.2. ExperimentalBefore deposition, N-type Si (1 0 0) wafers with a resistivity of (1-10) Ω- cm were cleaned by a modified RCAprocess, (using ultrasonic bath into different chemicals such as, acetone, alcohol and di-ionized water for 5 minuteseach. To remove any native oxide and hydrogen passivity on the surface, substrate was dipped in 1% buffered Hfsolution. Cleaned substrates were dried by N2 and put into the deposition chamber of JGP450 vacuum magnetronsputtering equipment. The deposition was performed under a mixture of Argon (Ar) and oxygen (O2) ambientsupplied as reactive gases, respectively. Hafnium disk of 99.99% purity with the diameter of 60 mm was used as thesputtering main target, while other targets titanium and erbium were fixed on the main target disk. The sputteringchamber was evacuated with lowest pressure about 3 ×10−4Pa before Ar and O2 gases were used. The target waspre-sputtered in argon (Ar) ambient for 10 min in order to remove surface oxide on the target, prior to HfTiErOdeposition. During the deposition process, the RF power, substrate temperature, working pressure, substrate-to-target distance, total gas-flow rate were kept at 100 W, 250 °C, 0.7 Pa, 5.5 cm, and 0.4 ratio, respectively. In order toobtain HfTiErO films with different Ti and Er contents. There is different Ti and Er materials were introduced onHafnium oxides, after deposition the ultra thin films were annealed in N2 atmosphere for 60 s at 500 °C and 700 °Ctemperatures.2.1 C-V CharacterizationsElectrical properties of the MOS capacitor were measured using a using HP 4294A LCR meter, impedance/gain-phase analyzer. CET was extracted from an accumulation capacitance measured at 1MHz, without deducting for thequantum mechanical effect. The voltage of the external signal is 30mV and the external DC bias scanning with theorder of -4V—> +4V—> -4V.2.2 AFM and XPS characterizationThe microstructure and chemical composition of the deposited material were characterized by using AFM and XPS.In the work the primitive CSPM5000 series of scanning probe microscopy used to analysis the sample’s film surfacemorphology, while Chemical composition of the elements were made at The Experimental Analysis Center,Tsinghua University by X-ray photoelectron spectroscopy (XPS) using PHI Quantera SXM with 45°take-off angle.3. Result and discussions3.1 Atomic force microscopy (AFM)The AFM research on the surface roughness to check the surface morphology of both as-deposited and annealedfilms, especially high-k materials, appears very significant because this is an important physical property that mayaffect the electrical properties of dielectric thin films and induces shifts in electronic energy levels (Song et al., 2007)and (Tao et al., 2011). To expose the relationship between the doping content of Er and surface morphology theAFM images were taken for all samples as deposited and in N2 ambient at 500 °C and 700 °C for 60 s and are shownin Fig. 1. The samples were scanned at the size of 2 × 2 μm. It can be observed from the results that the surfaceroughness of films is improved slightly by increasing the Er concentration. The results demonstrated that the filmsdisplay a homogeneous and smooth surface structure, by means of a homogeneous material distribution with a lowsurface roughness after the provide annealing temperatures at 500 °C and 700 °C. The AFM analysis of both asdeposited and annealed films show the root mean square (RMS) surface roughness calculated from the AFM imagesfor S1, S2, S3, S4 and S5 are approximately 5.0nm, 4.0nm, 3.8nm, 3.0nm and 3.2nm, respectively. It is remarkableto find that the surface of S1 and S2 samples consist of dense narrow spikes in shape, whereas the samples S4 and S5are more mountain like, flat and void free. This spiky augment in roughness for S2 and S3 is possibly attributed to atransformation of phase structure. It was also reported that the amorphous structure of the thin film is changed intothe polycrystalline structure after annealing; due to the increase of the grain size will result in an increase of the
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201343surface roughness (Cho et al., 2006). This may shows that the surface of films acquires smoother after annealingprocess. The diffusion and mobility of the surface atoms can be increased by increasing the annealing temperature,which provides energy to surface atoms. Due to transfer of such atoms to existing voids and defects, the surface getssmoother and reduces the surface roughness3.2 XPSThe Chemical compositions of the elements were made by using X-ray photoelectron spectroscopy (XPS) using PHIQuantera SXM with 45°take-off angle. The XPS profiles for the samples (1), (2), (3), (4) and (5) (S1-HfTi6O, S2-HfTi6Er2O, S3-HfTi6Er4O, S4-HfTi6Er4O at 500℃ and S5-HfTi6Er4O at 700℃) are shown in Fig.2. It can be seenthat a series of peaks from Hf4f, Er4d, Hf4d, C1s, Ti2p and O1s arisen from the surface contamination ofadventitious carbon are clearly observed. Annealing leads to the removal of C1s peaks for the samples (2) and (4).Effects of experimental charging were corrected by setting the C1s peak for adventitious carbon at 284.6 eV. Thedifferent percentage ratios of the content were analysis and are shown in table.1.3.3 MOS fabrications and C-V measurements:The MOS structure of the gate dielectric is helpful to understand the various electrical characteristics of the high-kdielectric materials, such as the relative permittivity of the high-k dielectric, there are various charge defects insidethe thin film and the Si substrate contact interface characteristics and so on. However, to investigate the impact of Tiand Er addition in HfO2 films, capacitors with MOS electrodes were fabricated. Fig.3 showed well-behavedcapacitance-voltage (C-V) curves for the target of HfTiErO films at different Er contents. All HfTiErO films,regardless of their Er content, have a nominal flat band voltage (Vfb) shift relative to the HfTiO while sampleHfTi6Er4O shows the highest capacitance density relative to the rest of the other samples. Whereas from the C-Vcures it can be seen that the geometry of all as deposited sample curves is not symmetric possibly due to the ultrathin thickness which might be caused of leakage current. The detailed analysis of the different value of Er dopedHfTiO films at different Er contents. Results indicate that of all the different Er contents, HfTiO is the not mostpromising on substrate temperatures. The films have the highest leakage of current.3.4 Annealed C-V curves.Fig.4 demonstrates high frequency C-V characteristics of annealed HfTiErO gate dielectric MOS capacitors.According to the accumulation capacitance, it can be seen that the film annealed at 500 °C has improved electricalproperties as compare to without annealed samples.It can be seen that films annealed temperature at 500 °C has the improved Electrical properties, almost samples havevery high k dielectric constant may be resulted from the microstructure change such as crystalline. We also obtainedthe flat band voltage (Vfb) from C-V curves. Vfb primarily depends on deficiencies in HfTiErO film and theinterface traps at the interface. The interfacial layer is formed unavoidably and after annealing the thickness of thefilm decreased, the reason lies in that with the increase of temperature, SiOx in gradually converted into silicate bythe reaction of between HfTiErO and SiOx. The Ultrathin HfTiErO films annealed at 500 °C in nitrogen atmospheretemperature interfacial SiOx completely converted into silicate, which explained in many previous literatures (Ye etal., 2010).According to the accumulative capacitance, the dielectric constant k can be calculated. It can be seen that at sampleHfTi6Er4O has the highest k value of 30.0 as compare to other samples. This may be due to the SiOx completelyconverted into silicate, which demonstrated good interfacial quality (Ye et al., 2011) . The permittivity valueextracted from 1 MHz C-V curves are usually underestimated due to the well-known effect of series resistance on thecapacitance at accumulation which is stronger at higher frequencies (Li et al., 2008). All sample having goodelectrical properties although the sample HfTi6Er4O films achieved best electrical properties as compare othersamples.5. ConclusionIn summary, a higher-k material HfTiErO has been demonstrated. Its amorphous structure is sustained up to a postannealing temperature of 500 °C. By incorporating TiO2 and Er2O3, the dielectric constant could be increased withother electrical properties. Moreover, XPS Hf 4f and O1 s results can be concluded that ultra thin HfTiErO filmsmicrostructure is formed, while the anealed temperature also effected on the the microsturuture that caused theincrease in intensity and binding energy as well. These improved material and electrical results indicate that HfTiErOmay be a promising candidate for the next generation of higher-k gate dielectrics.
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201344ReferencesSchaller RR. Technological innovation in the semiconductor industry: A case study of the international technologyroadmap for semiconductors (ITRS). thesis. George Mason University, 2004Wilk GD, Wallace RM, Anthony JM. High-κ gate dielectrics: Current status and materials properties considerations.Journal of Applied Physics, 2001, 89: 5243Akbar MS, Gopalan S, Cho H-J, et al. High-performance TaN/HfSiON/Si metal-oxide-semiconductor structuresprepared by NH3 post-deposition anneal. Applied Physics Letters, 2003, 82: 1757-1759Mikhelashvili V, Eisenstein G, Edelmann F. Characteristics of electron-beam-gun-evaporated Er2O3 thin films asgate dielectrics for silicon. Journal of Applied Physics, 2001, 90: 5447Buchanan D. Scaling the gate dielectric: Materials, integration, and reliability. IBM journal of research anddevelopment, 1999, 43: 245-264Yamamoto Y, Kita K, Kyuno K, et al. Structural and electrical properties of HfLaOx films for an amorphous high-kgate insulator. Applied Physics Letters, 2006, 89: 032903Chen F, Bin X, Hella C, et al. A study of mixtures of HfO2 and TiO2 as high-k gate dielectrics. MicroelectronicEngineering, 2004, 72: 263-266Auciello O, Fan W, Kabius B, et al. Hybrid titanium–aluminum oxide layer as alternative high-k gate dielectric forthe next generation of complementary metal–oxide–semiconductor devices. Applied Physics Letters, 2005, 86:042904-042904-042903Först CJ, Schwarz K, Blöchl PE. Structural and electronic properties of the interface between the high-k oxideLaAlO3 and si (001). Physical review letters, 2005, 95: 137602Klie R, Browning N, Chowdhuri AR, et al. Analysis of ultrathin SiO interface layers in chemical vapor deposition ofAlO on Si by in situ scanning transmission electron microscopy. Applied Physics Letters, 2003, 83: 1187Kim J, Yong K. Characterization of hafnium silicate thin films grown by MOCVD using a new combination ofprecursors. Journal of Crystal Growth, 2004, 263: 442-446Dey S, Das A, Tsai M, et al. Relationships among equivalent oxide thickness, nanochemistry, and nanostructure inatomic layer chemical-vapor-deposited Hf–O films on Si. Journal of Applied Physics, 2004, 95: 5042-5048Park BK, Park J, Cho M, et al. Interfacial reaction between chemically vapor-deposited hfo thin films and a Hf-cleaned Si substrate during film growth and postannealing. Applied Physics Letters, 2002, 80: 2368He G, Zhu L, Liu M, et al. Optical and electrical properties of plasma-oxidation derived HfO2 gate dielectric films.Applied Surface Science, 2007, 253: 3413-3418Ergin FB, Turan R, Shishiyanu ST, et al. Effect of γ-radiation on HfO2 based MOS capacitor. Nuclear Instrumentsand Methods in Physics Research Section B: Beam Interactions with Materials and Atoms, 2010, 268: 1482-1485Song X, Takoudis CG. Cyclic chemical-vapor-deposited TiO2/Al2O3 film using trimethyl aluminum, tetrakis(diethylamino) titanium, and O2. Journal of The Electrochemical Society, 2007, 154: G177-G182Tao Q, Kueltzo A, Singh M, et al. Atomic layer deposition of HfO2, TiO2, and HfxTi1-xO2 using metal (diethylamino)precursors and HfO2. Journal of The Electrochemical Society, 2011, 158: G27-G33Cho D-Y, Oh S-J, Chang Y, et al. Role of oxygen vacancy in HfO2/SiO2/Si (100) interfaces. Applied Physics Letters,2006, 88: 193502-193502-193503Ye C, Wang H, Zhang J, et al. Composition dependence of band alignment and dielectric constant for Hf1−xTixO2thin films on si (100). Journal of Applied Physics, 2010, 107: 104103Ye C, Wang Y, Zhang J, et al. Evidence of interface conversion and electrical characteristics improvement of ultra-thin HfTiO films upon rapid thermal annealing. Applied Physics Letters, 2011, 99: 182904-182904-182903Li CX, Zou X, Lai PT, et al. Effects of Ti content and wet-N2 anneal on Ge MOS capacitors with HfTiO gatedielectric. Microelectronics Reliability, 2008, 48: 526-530Murad Ali Khaskheli was born in Sindh Province, Pakistan, in August 1976. He received hisM.Sc. degrees in Physics from Sindh University of, Jamshoro, He is working as a Lecturer atfaculty of Sciences, Institute of Physics, University of Sindh, Jamshoro since August 2003.Recently he is pursuing PhD degree in Department of Physics and Mathematics, University ofScience and Technology Beijing P. R. China. His research interests are in hafnium baseddielectric materials.
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201345Prof Wu Ping was born in P.R China. Received Ph.D degree from University of Science andTechnology Beijing. In 1982-1984 work at China Academy of Engineering Physics Institute ofApplied Physics and Computational Mathematics. 1993-1994 study in the United States. She isPh.D supervisor and deputy director of Department of Physics and Mathematics University ofscience and technology Beijing.Amir Mahmood Soomro was born in Sindh Province, Pakistan, in March 1984. He received hisB.E. and M.E. degrees in Electrical Engineering from Mehran University of Engineering andTechnology, Jamshoro, in 2006 and 2010, respectively.He joined the faculty of Electrical, Electronics and Computer System Engineering (FEECE),Mehran University of Engineering and Technology (MUET), Jamshoro, in March 2006. He wasworking as a Lecturer in department of Electrical Engineering, MUET, Jamshoro till August 2010. Recently he is onstudy leave for pursuing PhD degree. He is studying in School of Automation, Beijing Institute of Technology, P. R.China. He is the member of Pakistan Engineering Council (PEC) since 2006. His research interests are in PowerQuality, Network Topologies, Power Electronics and Control.Dr. Matiullah Khan was born in KPK province, Pakistan getting master degree in physics; He joined university ofscience and technology Banu KPK, Pakistan as a Lecturer in Physics. Dr. Khan mainly works on two projects. Thefirst one deals with the synthesis of novel visible light active TiO2 photocatalysts. This includes the band structuretuning, electronic band structure investigation, optical and photocatalytic properties. Mainly Dr. Khan focus on TiO2based materials. The second field of interest is the ab-initio calculations for investigating the structural, electronicand optical properties of various semiconductors.Prof. Mohammad Siddique Kalhoro was born in Sindh Province, Pakistan. Ph.D in Condensed Matter andMaterial Physics (1999) from London UK M.Sc Physics (1987) Institute of Physics, University of Sindh,Jamshoro B.Sc Physics (1985) Institute of Physics, University of Sindh, Jamshoro Recently working as Professorand Pro Vice Chancellor University of Sindh, Jamshoro,Pakistan.Figure 1. AFM surface images (2 × 2 μm) of different samples as deposited and annealed
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201346Figure 2. Typical XPS spectrum of as grown and annealed samplesFigure 3. C-V curves of Er doped HfTiO films at different Er contents